General

Property | Value | Condition | Shape |
---|---|---|---|

Density | 2.81 g/cm³ Show Material materials with Density of 2.81 g/cm³ | T651 | |

2.81 g/cm³ Show Material materials with Density of 2.81 g/cm³ | T651 | Bar | |

3.1 g/cm³ Show Material materials with Density of 3.1 g/cm³ | T651 |

Mechanical

Property | Temperature | Value | Condition | Related Standards | Shape | Comment |
---|---|---|---|---|---|---|

Bending Fatigue Strength | 160.0 MPa Show Material materials with Bending Fatigue Strength of 160.0 MPa | T651 | AA Standards | |||

Compressive modulus | 72.4 MPa Show Material materials with Compressive modulus of 72.4 MPa | T651 | ||||

Elastic modulus | 72.0 GPa Show Material materials with Elastic modulus of 72.0 GPa | T651 | Bar | |||

Elongation | -195 °C | 9 % Show Material materials with Elongation of 9 % | T651 | Elongation in 50 mm | ||

-80 °C | 11 % Show Material materials with Elongation of 11 % | T651 | Elongation in 50 mm | |||

2.0 % Show Material materials with Elongation of 2.0 % | T651 | AA Standards, ASTM B209 | A100 | |||

4.0 % Show Material materials with Elongation of 4.0 % | T651 | AA Standards, ASTM B209 | A100 | |||

5.0 % Show Material materials with Elongation of 5.0 % | T651 | AA Standards, ASTM B209 | A100 | |||

6.0 % Show Material materials with Elongation of 6.0 % | T651 | AA Standards, ASTM B209 | A100 | |||

7.0 % Show Material materials with Elongation of 7.0 % | T651 | AA Standards, ASTM B211 | Bar | A50 | ||

7.4 % Show Material materials with Elongation of 7.4 % | T651 | |||||

9.0 % Show Material materials with Elongation of 9.0 % | T651 | AA Standards, ASTM B209 | A50 | |||

9.0 % Show Material materials with Elongation of 9.0 % | T651 | AA Standards | A100 | |||

11.0 % Show Material materials with Elongation of 11.0 % | T651 | AA Standards | A50 | |||

11.0 % Show Material materials with Elongation of 11.0 % | T651 | |||||

0 °C | 11 % Show Material materials with Elongation of 11 % | T651 | Elongation in 50 mm | |||

24 °C | 11 % Show Material materials with Elongation of 11 % | T651 | Elongation in 50 mm | |||

100 °C | 14 % Show Material materials with Elongation of 14 % | T651 | Elongation in 50 mm | |||

150 °C | 30 % Show Material materials with Elongation of 30 % | T651 | Elongation in 50 mm | |||

205 °C | 55 % Show Material materials with Elongation of 55 % | T651 | Elongation in 50 mm | |||

260 °C | 65 % Show Material materials with Elongation of 65 % | T651 | Elongation in 50 mm | |||

315 °C | 70 % Show Material materials with Elongation of 70 % | T651 | Elongation in 50 mm | |||

370 °C | 70 % Show Material materials with Elongation of 70 % | T651 | Elongation in 50 mm | |||

Fatigue strength | 159 MPa Show Material materials with Fatigue strength of 159 MPa | T651 | for 5x10⁸ cycles | |||

Hardness, Brinell | 150.0 [-] Show Material materials with Hardness, Brinell of 150.0 [-] | T651 | AA Standards | |||

150.0 [-] Show Material materials with Hardness, Brinell of 150.0 [-] | T651 | 500 kg load, 10 mm ball | ||||

Plane-Strain Fracture Toughnes | -196 °C | 33.5 MPa·√m Show Material materials with Plane-Strain Fracture Toughnes of 33.5 MPa·√m | T651 | For plate in T-L direction | ||

24.2 MPa·√m Show Material materials with Plane-Strain Fracture Toughnes of 24.2 MPa·√m | T651 | |||||

24 °C | 32.3 MPa·√m Show Material materials with Plane-Strain Fracture Toughnes of 32.3 MPa·√m | T651 | For plate in T-L direction | |||

Unlock all property charts | ||||||

Poisson's ratio | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | T651 | ||||

Shear modulus | 26.9 GPa Show Material materials with Shear modulus of 26.9 GPa | T651 | ||||

Shear strength | 331.0 MPa Show Material materials with Shear strength of 331.0 MPa | T651 | ||||

Tensile strength | -195 °C | 703 MPa Show Material materials with Tensile strength of 703 MPa | T651 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | ||

-80 °C | 620 MPa Show Material materials with Tensile strength of 620 MPa | T651 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | |||

460.0 MPa Show Material materials with Tensile strength of 460.0 MPa | T651 | AA Standards, ASTM B209 | ||||

490.0 MPa Show Material materials with Tensile strength of 490.0 MPa | T651 | AA Standards, ASTM B209 | ||||

495.0 MPa Show Material materials with Tensile strength of 495.0 MPa | T651 | AA Standards, ASTM B209 | ||||

505.0 MPa Show Material materials with Tensile strength of 505.0 MPa | T651 | AA Standards, ASTM B211 | ||||

515.0 MPa Show Material materials with Tensile strength of 515.0 MPa | T651 | AA Standards, ASTM B211 | ||||

525.0 MPa Show Material materials with Tensile strength of 525.0 MPa | T651 | AA Standards, ASTM B209 | ||||

530.0 MPa Show Material materials with Tensile strength of 530.0 MPa | T651 | AA Standards, ASTM B209, ASTM B211 | ||||

531.0 MPa Show Material materials with Tensile strength of 531.0 MPa | T651 | Bar | ||||

540.0 MPa Show Material materials with Tensile strength of 540.0 MPa | T651 | AA Standards, ASTM B209 | ||||

560.0 MPa Show Material materials with Tensile strength of 560.0 MPa | T651 | |||||

570.0 MPa Show Material materials with Tensile strength of 570.0 MPa | T651 | AA Standards | ||||

0 °C | 593 MPa Show Material materials with Tensile strength of 593 MPa | T651 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | |||

24 °C | 572 MPa Show Material materials with Tensile strength of 572 MPa | T651 | ||||

100 °C | 483 MPa Show Material materials with Tensile strength of 483 MPa | T651 | ||||

150 °C | 215 MPa Show Material materials with Tensile strength of 215 MPa | T651 | ||||

205 °C | 110 MPa Show Material materials with Tensile strength of 110 MPa | T651 | ||||

260 °C | 75 MPa Show Material materials with Tensile strength of 75 MPa | T651 | ||||

315 °C | 55 MPa Show Material materials with Tensile strength of 55 MPa | T651 | ||||

370 °C | 40 MPa Show Material materials with Tensile strength of 40 MPa | T651 | ||||

Unlock all property charts | ||||||

Yield strength | -196 °C | 634 MPa Show Material materials with Yield strength of 634 MPa | T651 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | ||

-80 °C | 545 MPa Show Material materials with Yield strength of 545 MPa | T651 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | |||

-28 °C | 517 MPa Show Material materials with Yield strength of 517 MPa | T651 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | |||

370.0 MPa Show Material materials with Yield strength of 370.0 MPa | T651 | AA Standards, ASTM B209 | RP02 | |||

400.0 MPa Show Material materials with Yield strength of 400.0 MPa | T651 | AA Standards, ASTM B209 | RP02 | |||

420.0 MPa Show Material materials with Yield strength of 420.0 MPa | T651 | AA Standards, ASTM B209 | RP02 | |||

425.0 MPa Show Material materials with Yield strength of 425.0 MPa | T651 | AA Standards, ASTM B211 | RP02 | |||

440.0 MPa Show Material materials with Yield strength of 440.0 MPa | T651 | AA Standards, ASTM B209, ASTM B211 | RP02 | |||

455.0 MPa Show Material materials with Yield strength of 455.0 MPa | T651 | AA Standards, ASTM B211 | Bar | RP02 | ||

460.0 MPa Show Material materials with Yield strength of 460.0 MPa | T651 | AA Standards, ASTM B209 | RP02 | |||

470.0 MPa Show Material materials with Yield strength of 470.0 MPa | T651 | AA Standards, ASTM B209 | RP02 | |||

470.0 MPa Show Material materials with Yield strength of 470.0 MPa | T651 | |||||

505.0 MPa Show Material materials with Yield strength of 505.0 MPa | T651 | AA Standards | RP02 | |||

505.0 MPa Show Material materials with Yield strength of 505.0 MPa | T651 | |||||

24 °C | 503 MPa Show Material materials with Yield strength of 503 MPa | T651 | ||||

100 °C | 448 MPa Show Material materials with Yield strength of 448 MPa | T651 | ||||

149 °C | 186 MPa Show Material materials with Yield strength of 186 MPa | T651 | ||||

204 °C | 87 MPa Show Material materials with Yield strength of 87 MPa | T651 | ||||

260 °C | 62 MPa Show Material materials with Yield strength of 62 MPa | T651 | ||||

316 °C | 45 MPa Show Material materials with Yield strength of 45 MPa | T651 | ||||

371 °C | 32 MPa Show Material materials with Yield strength of 32 MPa | T651 | ||||

Unlock all property charts |

Thermal

Property | Value | Condition | Shape |
---|---|---|---|

Coefficient of thermal expansion | 2.3e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.3e-05 1/K | T651 | |

2.35e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.35e-05 1/K | T651 | Bar | |

Melting point | 477.0 °C Show Material materials with Melting point of 477.0 °C | T651 | |

480.0 °C Show Material materials with Melting point of 480.0 °C | T651 | ||

635.0 °C Show Material materials with Melting point of 635.0 °C | T651 | Bar | |

Specific heat capacity | 910.0 J/(kg·K) Show Material materials with Specific heat capacity of 910.0 J/(kg·K) | T651 | |

Thermal conductivity | 130.0 W/(m·K) Show Material materials with Thermal conductivity of 130.0 W/(m·K) | T651 | |

134.0 - 160.0 W/(m·K) Show Material materials with Thermal conductivity of 134.0 - 160.0 W/(m·K) | T651 | Bar |

Electrical

Property | Value | Condition | Shape | Comment |
---|---|---|---|---|

Electrical conductivity | 19000000 S/m Show Material materials with Electrical conductivity of 19000000 S/m | T651 | Typical/derived value | |

Electrical resistivity | 4.31e-08 Ω·m Show Material materials with Electrical resistivity of 4.31e-08 Ω·m | T651 | Bar | |

5.22e-08 Ω·m Show Material materials with Electrical resistivity of 5.22e-08 Ω·m | T651 | Typical value | ||

Specific Electrical conductivity | 33.0 % IACS Show Material materials with Specific Electrical conductivity of 33.0 % IACS | T651 | Typical value |

Chemical properties

Property | Value | Condition | Related Standards | Shape | Comment |
---|---|---|---|---|---|

Aluminium | 86.9 - 91.4 % Show Material materials with Aluminium of 86.9 - 91.4 % | T651 | |||

Chromium | 0.18 - 0.28 % Show Material materials with Chromium of 0.18 - 0.28 % | T651 | AA Standards, ASTM B209, ASTM B211 | Bar | |

Copper | 1.2 - 2.0 % Show Material materials with Copper of 1.2 - 2.0 % | T651 | AA Standards, ASTM B209, ASTM B211 | Bar | |

Iron | 0.50 % Show Material materials with Iron of 0.50 % | T651 | AA Standards, ASTM B209, ASTM B211 | ||

0.5 % Show Material materials with Iron of 0.5 % | T651 | Bar | |||

Magnesium | 2.1 - 2.9 % Show Material materials with Magnesium of 2.1 - 2.9 % | T651 | AA Standards, ASTM B209, ASTM B211 | Bar | |

Manganese | 0.3 % Show Material materials with Manganese of 0.3 % | T651 | AA Standards, ASTM B209, ASTM B211 | Bar | |

Other | 0.15 % Show Material materials with Other of 0.15 % | T651 | Bar | Total | |

Silicon | 0.4 % Show Material materials with Silicon of 0.4 % | T651 | AA Standards, ASTM B209, ASTM B211 | Bar | |

Titanium | 0.2 % Show Material materials with Titanium of 0.2 % | T651 | AA Standards, ASTM B209, ASTM B211 | Bar | |

Zinc | 5.1 - 6.1 % Show Material materials with Zinc of 5.1 - 6.1 % | T651 | AA Standards, ASTM B209, ASTM B211 | Bar | |

Zirconium | 0.25 % Show Material materials with Zirconium of 0.25 % | T651 |

Technological properties

Property | ||
---|---|---|

Brazing | general: no brazing is known or developed | |

Corrosion properties | Stress corrosion cracking: Operational damage in areas with tensile stresses transverse to the grain structure, limited damage to laboratory samples, general: good, without protection in industrial or seawater atmosphere | |

General machinability | General: poor (O), good to acceptable | |

Workability | general (condition): not suitable |